Ceramics and glass materials
Embed Size (px)
Transcript of Ceramics and glass materials
Ceramic and Glass Materials
Structure, Properties and Processing
James F. Shackelford Robert H. DoremusEditors
Ceramic and Glass Materials
Structure, Properties and Processing
EditorsJames F. Shackelford Robert H. DoremusUniversity of California, Davis Materials Research CenterDept. Chemical Engineering Rensselaer Polytechnic Institute & Materials Science Dept. Materials Science & Engineering1 Shields Avenue 110 8th StreetDavis, CA 95616 Troy, NY 12180-3590
ISBN 978-0-387-73361-6 e-ISBN 978-0-387-73362-3DOI 10.1007/978-0-387-73362-3
Library of Congress Control Number: 2007938894
2008 Springer Science+Business Media, LLCAll rights reserved. This work may not be translated or copied in whole or in part without the written permission of the publisher (Springer Science+Business Media, LLC, 233 Spring Street, New York, NY 10013, USA), except for brief excerpts in connection with reviews or scholarly analysis. Use in connection with any form of information storage and retrieval, electronic adaptation, computer software, or by similar or dissimilar methodology now known or hereafter developed is forbidden. The use in this publication of trade names, trademarks, service marks, and similar terms, even if they are not identifi ed as such, is not to be taken as an expression of opinion as to whether or not they are subject to proprietary rights.
Printed on acid-free paper
9 8 7 6 5 4 3 2 1
Robert H. Doremus A Dedication
With sadness, I note that in late January 2008 while finishing the editing of this book, Bob Doremus passed away suddenly in Florida. His wife and one of his daughters were with him at the time. Characteristic of his meticulous attention to detail, he had just finished personally preparing the index for this volume. Professor Doremus was an icon of ceramic and glass science, and this volume is a fitting tribute to his career. In addition to editing the book, he provided the opening chapter on alumina, the quin-tessential structural ceramic material.
After finishing two Ph.D. degrees in physical chemistry (University of Illinois, 1953 and University of Cambridge, 1956), Dr. Doremus worked at the General Electric Research and Development Laboratory for many years during a period of time that can fairly be described as a golden age of ceramic and glass science. His colleagues included Robert Coble, Joseph Burke, and Paul Jorgensen. There, he con-ducted seminal research including classic studies of gas and water diffusion in ceram-ics and glasses.
In 1971, he moved to the Department of Materials Science and Engineering at the Rensselaer Polytechnic Institute and began a long career as an educator. He continued to work on a broad range of topics in ceramic and glass science and was especially well known for publishing the definitive version of the important alumina-silica phase diagram [Klug, Prochazka, and Doremus, J.Am.Ceram.Soc., 70 750 (1987)] as well as doing pioneering work on bioceramics for medical applications. At Rensselaer, Bob was named the New York State Science and Technology Foundation Professor of Glass and Ceramics and served as Department Chair from 1986 to 1995.
Appropriate to his distinguished career as a scientist and educator, Bob received numerous awards in recognition of his accomplishments. Resulting in nearly 300 publi-cations, his research contributions were recognized with the Scholes Award of Alfred University, the Morey Award of the American Ceramic Society, and the Ross Coffin Purdy Award, the American Ceramic Societys top honor for research. He received numerous teaching awards while at Rensselaer, including the Outstanding Educator Award of the American Ceramic Society. His winning the top research and educator awards of the American Ceramic Society is symbolic of his remarkable career.
Beyond these professional accomplishments of a great scientist and dedicated teacher, Bob Doremus was a devoted family man and leaves behind his wife Germaine
and children Carol, Elaine, Mark, and Natalie. As with his family, Bob cared deeply about his students and worked tirelessly to help them. He was also a fine and support-ive colleague. He will be greatly missed, and this book is dedicated to him with both affection and respect.
J.F. ShackelfordDavis, CA
vi Robert H. Doremus A Dedication
This book is intended to be a concise and comprehensive coverage of the key ceramic and glass materials used in modern technology. A group of international experts have contributed a wide ranging set of chapters that literally covers this field from A (Chap. 1) to Z (Chap. 10). Each chapter focuses on the structureproperty relationships for these important materials and expands our understanding of their nature by simultaneously discussing the technology of their processing methods. In each case, the resulting understanding of the contemporary applications of the materials provides insights as to their future role in twenty-first century engineering and technology.
The book is intended for advanced undergraduates, graduate students, and working professionals. Although authored by members of the materials science and engineer-ing community, the book can be useful for readers in a wide range of scientific and engineering fields.
Robert Doremus of the Rensselaer Polytechnic Institute covers one of the most ubiquitous modern ceramics in Chap. 1. The popularity of alumina by itself and as a component in numerous ceramic and glass products follows from its wide range of attractive properties. In Chap. 2, Duval, Risbud, and Shackelford of the University of California, Davis, look at the closely related and similarly ubiquitous material com-posed of three parts of alumina and two parts of silica, the only stable intermediate phase in the aluminasilica system at atmospheric pressure. Mullite has had significant applications in refractories and pottery for millennia and new applications in struc-tures, electronics, and optics are the focus of active research. Richard Bradt of the University of Alabama, Tuscaloosa, provides Chap. 3, a focused discussion of the intriguing minerals (andalusite, kyanite, and sillimanite) that do not appear on the common aluminasilica phase diagram as they are formed at high geological pressures and temperatures. Nonetheless, these minerals with a one-to-one ratio of alumina to silica are widely found in nature and are used in numerous applications such as refrac-tories for the steel and glass industries. In Chap. 4, Martin Wilding of the University of Wales, Aberystwyth, further expands the compositional range of materials considered by exploring the ceramics and glasses formed in binary aluminate systems. Sharing the high melting point and chemical resistance of the alumina end-member, these aluminates find a wide range of applications from cements to bioceramics and electronic components.
In Chap. 5, Davila, Risbud, and Shackelford of the University of California, Davis, review the various ceramic and glass materials that come from silica, the most abundant mineral in the Earths crust. The many examples they give share a simple chemistry but display a wide range of crystalline and noncrystalline structures. The materials also represent some of the most traditional ceramic and glass applications as well as some of the most sophisticated, recent technological advances. In Chap. 6, Smith and Fahrenholtz of the University of Missouri, Rolla, cover a vast array of ceramic materials, including many of the materials covered in other chapters in this book. The resulting perspective is useful for appreciating the context in which ceramics are used for one of their most important properties, viz. the resistance to high temperatures. Professor Fahrenholtz then provides a comprehensive coverage of clays in Chap. 7. These important minerals that serve as raw materials for so many of the traditional ceramics are also providing a framework for the science of the study of advanced ceramics. In Chap. 8, Mariano Velez of the Mo-Sci Corporation reviews the ceramic oxides that are used for the two distinctive markets of (a) structural applica-tions and (b) high temperature (refractory) concretes.
Professor Julie Schoenung of the University of California, Davis, reviews a wide range of minerals in Chap. 9. These materials produce the various lead oxides and silicates so widely used in lead-containing glasses and crystalline electronic ceramics. The regulatory issues surrounding these well known carcinogenic materials are also discussed. Finally in Chap. 10, Olivia Graeve of the University of Nevada, Reno, reviews the complex structural and processing issues associated with the family of ceramics zirconia that is widely used because of the superior values of toughness and ionic conductivity.
Finally, we thank the staff of Springer for their consistent encouragement and professional guidance in regards to this book. We especially appreciate Gregory Franklin for helping to initiate the project and Jennifer Mirski for guiding it to completion.
Davis, CA ShackelfordTroy, NY Doremus
Preface. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . vii
Contributors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . xi
Chapter 1 Alumina . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1Robert H. Doremus
Chapter 2 Mullite . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 27David J. Duval, Subhash H. Risbud, and James F. Shackelford
Chapter 3 The Sillimanite Minerals: Andalusite, Kyanite, and Sillimanite . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 41Richard C. Bradt
Chapter 4 Aluminates. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 49Martin C. Wilding
Chapter 5 Quartz and Silicas . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 71Lilian P. Davila, Subhash H. Risbud, and James F. Shackelford
Chapter 6 Refractory Oxides. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 87Jeffrey D. Smith and William G. Fahrenholtz
Chapter 7 Clays. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 111William G. Fahrenholtz
Chapter 8 Concrete and Cement. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 135Mariano Velez
Chapter 9 Lead Compounds . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 151Julie M. Schoenung
Chapter 10 Zirconia . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 169Olivia A. Graeve
Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 199
Richard C. BradtDepartment of Materials Engineering, The University of Alabama, Tuscaloosa, AL 35487-0202, USA, [email protected]
Lilian P. DavilaDepartment of Chemical Engineering and Materials Science, University of California, Davis, CA 95616, USA, [email protected]
Robert H. DoremusDepartment of Materials Science and Engineering, Rensselaer Polytechnic Institute, Troy, NY, USA
David J. DuvalDepartment of Chemical Engineering and Materials Science, University of California, Davis, CA 95616, USA, [email protected]
William G. FahrenholtzMaterials Science and Engineering Department, Missouri University of Science and Technology, Rolla, MO 65409, USA, [email protected]
Olivia A. GraeveDepartment of Chemical and Metallurgical Engineering, University of Nevada, Reno, NV, USA, [email protected]
Subhash H. RisbudDepartment of Chemical Engineering and Materials Science, University of California, Davis, CA 95616, USA, [email protected]
Julie M. SchoenungDepartment of Chemical Engineering and Materials Science, University of California, Davis, CA 95616, USA, [email protected]
James F. ShackelfordDepartment of Chemical Engineering and Materials Science, University of California, Davis, CA 95616, USA, [email protected]
Jeffrey D. SmithMaterials Science and Engineering Department, Missouri University of Science and Technology, Rolla, MO 65409, USA, [email protected]
Mariano VelezMo-Sci Corporation, Rolla, MO 65401, USA, [email protected]
Martin C. WildingInstitute of Mathematical and Physical Sciences, University of Wales, Aberystwyth, Ceredigion SY23 3BZ, UK, [email protected]
J.F. Shackelford and R.H. Doremus (eds.), Ceramic and Glass Materials: 1Structure, Properties and Processing. Springer 2008
Robert H. Doremus
The uses, processing, structure, and properties of alumina are summarized in this arti-cle. Various polymorphs of alumina and its phase relations with other oxides are described. The following properties are discussed: mechanical, thermal, thermody-namic, electrical, diffusional, chemical, and optical. Quantitative values for these properties are given in tables. The usefulness of alumina results from its high strength, melting temperature, abrasion resistance, optical transparency, and electrical resistiv-ity. Traditional uses of alumina because of these properties are furnace components, cutting tools, bearings, and gem stones; more recent applications include catalyst substrates, tubes for arc lamps, and laser hosts. Possible new uses of alumina are in electronic circuits, optical components, and biomaterials. Alumina fibers for compos-ites and optics must be pure, defect free, and cheap.
3) is one of the most important ceramic materials, both pure and as a
ceramic and glass component. Some uses of alumina are given in Table 1; an exhaustive and detailed description of many of these uses is given in . There are also extensive dis-cussions of uses of alumina in . Processing of alumina is discussed in both these refer-ences, and  has a summary of some properties of alumina. In writing this review, I have relied on material from these references. Anyone interested in more details of processing and properties of alumina should obtain  from the American Ceramic Society. Reference  is also available from the Society and has additional information on processing and uses of alumina. More recently, there have been two issues of the Journal of the American Ceramic Society devoted to alumina [3, 4]; these issues concentrate on defects and inter-faces, especially grain boundaries , grain growth, and diffusion in alumina .
The usefulness of alumina derives from a variety of its properties. It has a high melting temperature of 2,054C, and is chemically very stable and unreactive, leading to applications as high-temperature components, catalyst substrates, and biomedical implants. The hardness, strength, and abrasion resistance of alumina are among the highest for oxides, making it useful for abrasive materials, bearings,
2 R.H. Doremus
and cutting tools. The electrical resistance of alumina is high, so it is used pure and as a component in electrical insulators and components. Alumina has excellent optical transparency, and along with additives such as chromium and titanium, it is important as a gem stone (sapphires and rubies) and a laser host (ruby). Because of its high melting temperature, chemical inertness, and optical transparency, it is highly useful for containing arcs in street lamps. See Table 1 and also [1, 2] for more on uses of alumina.
In this review, the processing of alumina is discussed next, and then its properties are tabulated and described. In a summary future uses of alumina are considered.
2.1 Raw Materials
Bauxite is the name of the ore that is the primary source of alumina; bauxite contains gibbsite, -Al(OH)
3, which is the stable phase of Al(OH)
3 at ambient temperature and
pressure. The structure of alumina and hydrated alumina phases are listed in Table 2.
Table 1 Uses of Alumina
Furnace componentsCatalyst substratesElectronics substratesElectrical insulatorsCutting toolsBearingsSpark PlugsArc lamp tubesLaser hostsGem stones
Oxidation protection of aluminum and aluminum alloys
Thermal insulatorsFire retardation
Alumina as a component of
Ceramics and glassesMullite componentsElectrical insulatorsPorcelainsDurable glasses
1 Alumina 3
Bauxite from the Guianas in South America is low in iron and silica impurities, so it is preferred when purity is important. Other important sources of bauxite are in Brazil, the southern United States, Southeast Asia, West Africa, and India.
Aluminum hydroxides are separated from bauxite by the Bayer process, in which these hydroxides are dissolved in sodium hydroxide to separate them from the other unwanted constituents of the bauxite. The dissolution reactions are carried out at about 285C and 200 atm. pressure, and are:
Al(OH)3(s) + NaOH(soln) = NaAl(OH)
AlOOH(s) + H2O(soln) + NaOH(soln)= NaAl(OH)
in which (s) stands for solid and (soln) for solution. The solution containing NaAl(OH)4
is separated from the unwanted solid impurities by sedimentation and filtration, and the solute is cooled to about 55C. The aluminum hydroxides precipitate from the solution, aided by the addition of gibbsite seeds. The dried precipitated alumina or aluminum hydroxides can be used directly or further purified by resolution and reprecipitation. Other methods for preparing alumina and aluminum hydroxides from bauxite are described in [1, 2].
The stable phase of alumina at all temperatures and ambient pressure (one atm, or (1.01) 105 Pa) is corundum or -Al
3 (see Table 2). In single-crystal form, corun-
dum is called sapphire. No phase transformation of corundum up to 175 GPa pres-sure has been observed experimentally [5, 6]; however, a calculation predicts that corundum should transform to the Rh
3 (II) structure at about 78 GPa, and to a
cubic perovskite structure at 223 GPa . The Rh2O
3 (II) structure has an X-ray pat-
tern close to the corundum structure, so the transformation may have been missed in experimental studies.
Solid polycrystalline alumina is made from alumina powder by sintering. The traditional sintering methods for ceramics involve forming a powder into green ware, partially drying it at low temperatures, possibly calcining (heating) it at intermediate temperatures (perhaps 9001,100C), and firing it to a dense solid at high temperature, for alumina above 1,400C.
Table 2 Structures of stable alumina (corundum) and unstable aluminas
Lattice Parameters, angle ()
Designation Structure a b c
Corundum Hexagonal 4.758 12.991(rhombohedral)
Eta Cubic (spinel) 7.90 Gamma Tetragonal 7.95 7.79Delta Tetragonal 7.97 23.47Theta Monoclinic 5.63 2.95 11.86 103 42Kappa Orthorhombic 8.49 12.73 13.39
4 R.H. Doremus
The time and temperature required to form the desired degree of porosity in the dense solid depend mainly on the particle size of the alumina powder. The usual sintering sequence is imagined to be: (1) neck formation between powder particles, (2) formation of open porosity with a continuous solid phase (intermediate stage), and (3) removal of closed pores imbedded in the dense solid. In the usual practical sintering of alumina, stage one is rapid, and the final density or porosity is deter-mined mainly by stage three.
Various other oxides have been added to alumina to reduce the porosity of the final sintered solid. An especially valuable finding by Coble  was to add MgO to pure alumina powder; the resulting sintered alumina can be translucent (partial transmission of light). Usually sintered ceramics are opaque because of light scattering from residual pores, but in the translucent alumina, called Lucalox, the porosity is low enough to reduce this scattering, so that Lucalox tubes are used in street lamps for containing a sodium arc. Because the lamp can be operated at high temperature, it is quite efficient.
Dense alumina can also be made by melting, but the high-melting temperature of 2,054C makes this process expensive and difficult to control. High-value materials such as gem stones and laser hosts can be made by adding various colorants such as chromium, titanium, iron, cobalt, and vanadium to the melt.
In the sintering of alumina powders, the desired shape is formed in the green state before drying and firing. Various other constituents can be added to the starting powder. The density of the final product can be increased by hot-pressing, that is, by carrying out the firing under pressure. This method is expensive, so it is used only for high value polycrystalline products.
Alumina refractories for use in high temperature applications such as glass melting furnaces are usually made by the fusion-cast process. Various other oxides, such as SiO
2, MgO, Cr
3, and ZrO
2 are added to the alumina powder to
lower its melting point, and the resulting mixture is melted in an electric furnace and cast into the desired shapes for refractory applications. See the section on phase diagrams for the melting temperatures and compositions of a few mixtures of alumina with other oxides.
3 Structures of Pure and Hydrated Alumina
The structures of aluminas and hydrated aluminas are given in Tables 2 and 3. The only stable phase of Al
3 is corundum at all temperatures and up to at least 78 GPa pressure
(see earlier discussion). The corundum structure is shown in Fig. 1. It consists of oxy-gen ions in a slightly distorted close-packed hexagonal (rhombohedral) lattice, space group R3c. The aluminum ions occupy two-thirds of the octahedral sites in the oxygen lattice. The lattice parameters for corundum in Table 2 are for a hexagonal unit cell containing 12 Al
3 molecules. The rhombohedral lattice parameters are a = 5.128
and = 55.28. The ionic porosity Z of a solid is given by the formula
Z = 1- Va / V (3)
in which Va is the volume of atoms in a molecule (or in the unit cell) and V is the
specific volume, or the volume of the unit cell. For alumina Z = 0.21 with the radius
1 Alumina 5
of 1.38 for oxygen atoms, so the structure has less open volume even than close-packing (Z = 0.26) of uniform spheres.
The various metastable alumina structures are all less dense than corundum. Several other allotropic structures have been suggested, but are less well-verified than those in Table 2. All these metastable aluminas have oxygen packings that are near to close-packed cubic. Usually, eta or gamma aluminas are formed at low temperatures, and transform in the sequence gammadeltathetaalpha alumina with increasing temperatures. However, many other variants are possible, with gamma formed at higher temperatures and transforming directly to alpha. See  for some previous ref-erences. Factors such as particle size, heating rate, impurities, and atmosphere can influence the kinetics of transformation and the sequence of phases. Above about 1,200C, only alpha phase (corundum) is usually present.
The structures of various hydrated aluminas are given in Table 3. One configura-tion suggested for these structures is chains of AlO bonds with hydrogen bonding between chains. These hydrated aluminas decompose at low temperature (about 300C) to Al
3 and water.
Table 3 Structures of hydrated alumina phases
Lattice parameters ()/angle
Phase Formula A B c
Bayerite -Al(OH)3 Monoclinic 4.72 8.68 5.06/907
Gibbsite -Al(OH)3 Monoclinic 8.64 5.07 9.72/8526
Boehmite -AlOOH Orthorhombic 2.87 12.23 3.70Diaspore -AlOOH Orthorhombic 4.40 9.43 2.84
Fig. 1 The structure of alpha alumina from . The structure of corundum (alpha-alumina) from . The aluminum atoms occupy two-thirds of the octahedral interstices in a hexagonal close-packed array of oxygen atoms, which is distorted because the octahedral share faces in pairs
6 R.H. Doremus
4 Equilibrium Binary Phase Diagrams of Alumina with Other Oxides
The most important binary oxide and ceramic phase diagram is the aluminasilica (Al
2) diagram, shown in Fig. 2, as determined by Klug . Important fea-
tures in this diagram are the very low solid solubility of SiO2 in Al
3 and Al
SiO2 and the single stable intermediate solid phase of mullite, which has the com-
2; at higher temperatures, the amount of alumina in mullite
increases. In contrast to binary metal systems, which usually have considerable solid solubility in the pure components and limited solubility in intermetallic phases, there is some solid solubility in mullite and very little in the end members of SiO
2 (cristobalite) and Al
There is complete solid solubility in the system Al2O
3; both end members
have the corundum structure [11, 12]. There is also subsolidus phase separation in this system . There is also considerable solid solubility in the end-member oxides in the Al
3, and Al
3 systems . Thus, the
solid solubility results because the three-valent ions of Cr, Fe, Y, and Ga can substi-tute for aluminum in the corundum structure, and aluminum substitutes for these ions in their oxides. Alternatively, the solubilities of oxides with cation valences other than plus three are usually very low. For example, the solubility of magnesia in alumina is about 1 ppm atom fraction (Mg/Al) at 1,200C . Thus in mixtures of Al
3 with higher concentrations of MgO than 1 ppm, second phases containing
MgO can form on grain boundaries at 1,200C and lower temperatures, but the Mg atoms do not dissolve or substitute for Al in the Al
3. In the literature, there are
many reports of higher solubilities of ions with valences different from three in
SiO2 + MULLITE
0 20 4030 50 60 70 80 90 100
100 20 4030 50 60 70 80 90 100
Fig. 2 The aluminasilica phase diagram. From 
1 Alumina 7
alumina, but in view of the very careful work of Greskovitch and Brewer  with extremely pure alumina, these higher solubilities are unlikely.
In  there is a table (XI, on page 63) of minimum melting temperatures for a variety of binary alumina-oxide systems. With most oxides, these eutectic or peri-tectic temperatures vary from about 1,500 to 2,000C. The Al
5 system has
an anomalously low eutectic of 660C at 99% V2O
5; other low melting mixtures are
3 of 1,070C, Al
3 of 1,230C, and Al
3 of 1,440C.
5 Mechanical Properties
Alumina shows the deformation behavior of a typical brittle solid, which is linear elasticity to failure. Elastic deformation is instantaneous when stress is applied, and is completely reversible when it is removed. In a tensile test of a rod or bar of alumina, the strain is linear with stress to failure; the slope of this stressstrain curve is the Youngs modulus. Values of various moduli and Poissons ratio for pure, dense poly-crystalline alumina are given in Table 4 (from ). These values are considerably higher than those for most other oxides, as a result of the strong (high energy) alumi-numoxygen bonds in alumina. The various elastic constants of single crystal alumina are given in Table 5. As the temperature increases the elastic moduli decrease (as shown in Table 6) because of the increase in atomic displacements as the temperature increases, and consequent reduced bond strength.
Table 4 Elastic properties of polycrystalline alumina at room temperature , moduli in GPa
Youngs modulus 403Shear modulus 163Bulk modulus 254Poissons ratio 0.23
Table 5 Elastic properties of single crystal alumina at room temperature [2, 15] in GPa
C11 498 S11 23.5C12 163 S12 7.2C13 117 S13 3.6C14 23.5 S14 4.9C33 502 S33 21.7C44 147 S44 69.4
Table 6 Temperature dependence of Youngs modulus for polycrystalline alumina 
Temp. (C) Youngs modulus (GPa)
25 403500 3891,000 3731,200 364
8 R.H. Doremus
The mechanical strength of a brittle material such as alumina depends on flaws (cracks) in the alumina surface. When a tensile stress is applied perpendicular to a deep, thin crack, the stress at the tip of the crack is greatly magnified above the applied stress. Thus, the surface condition of a brittle solid determines it strength. Surface flaws develop from abrasion, so the higher the abrasion resistance of a brittle solid the greater its practical strength. Strengths of alumina are given in Table 7.
If a solid has no surface or internal flaws (a perfect lattice), it should have very high strength. Various theoretical equations for this ultimate strength S of a brittle solid have been proposed; one is 
S2 = Eg /4b (4)
in which E is Youngs modulus, g is the surface energy, and b the lattice parameter. With E = 403 GPa (Table 4), g = 6.0 J m2 [17, 18], and b = 0.177 nm, the ultimate strength S of alumina is about 58 GPa. This value is very high because of the high bond strength of alumina; for example, silicate glasses and quartz have theoretical strength values of 18 GPa or lower.
Practical strengths of brittle materials vary over wide ranges depending on their surface condition and history. For alumina, tensile or bonding strengths vary over a wide range of values because of different surface conditions, resulting in different flaw depths and flaw distributions. See  for a discussion of flaw distribution functions. The strength values for alumina are higher than for most other oxides; of course all of these strengths are far smaller than the theoretical strength, and depend strongly on the history and treatment of the samples. As the temperature increases, the strength of alumina decreases (as shown in Table 7) because of the increase of atomic vibrations and reduction in bond strength, just as for the reduction in elastic modulus with temperature. The strength of polycrystalline alumina depends strongly on its grain size, as shown by one set of strength values from . See also  for strengths of alumina machined and annealed at different temperatures. The strength also decreases as the alumina becomes more porous, as shown in Table 8; isolated pores increase the applied stress on their surfaces, and open porosity means much more surface for flaw development.
Table 7 Bend strengths of alumina in MPa
Theoretical strength 58,000 at 25C Ref.
Single crystals (sapphire) 300700 at 25C 2Polycrystals with similar treatment, 2
as a function of grain size in micrometers:Grain size 12 1015 4050 2Temp (C) 25C 460 330 240400C 360 260 2301,000C 340 260 2101,350C 260 110 97
1 Alumina 9
The strengths of crystalline and glassy oxides decrease with time under a constant applied load. This static fatigue is usually modeled with a power law equation between times to failure t when a sample is subjected to an applied stress s:
logt = c nlogs (5)
in which c is a constant and the stress exponent n is a measure of the susceptibility of the material to fatigue. The larger the n value the more resistant the material is to fatigue. Typical values of n for silicate glasses are 13 or lower ; for alumina an nvalue of about 35 was found , showing that alumina has much better fatigue resistance than most other oxides under ambient conditions.
This fatigue in oxides results from reaction with water, which can break the cationoxygen bonds in the material; for example in alumina:
Al O Al + H2O = AlOH + HOAl (6)
Thus, when the ambient atmosphere is dry the fatigue failure time is long, and as the humidity increases the fatigue time decreases.
The hardness of a material is measured by pressing a rod tip into a material and find-ing the amount of deformation from the dimensions of the resulting indentation. Hardness measurements are easy to make but hard to interpret. The stress distribution under the indenter is complex, and cracking, elastic and anelastic deformation, fault-ing, and plastic deformation are all possible around the indentation. Alumina is one of the hardest oxides. On the nonlinear Mohs scale of one to ten, alumina is nine and diamond is ten, but diamond is about a factor of three harder than alumina. Some approximate Knoop hardness (elongated pyramidal diamond indenter) values for alumina are given as a function of temperature in Table 9, and in Table 10 for some hard ceramics [22, 23]. It is curious that the hardness of alumina decreases much more than the strength as the temperature is increased.
Table 8 Effect of porosity on the bend strength of polycrystalline alumina at 25C from 
Porosity (%) Strength (MPa)
0 26910 17220 11030 7640 5550 47
10 R.H. Doremus
Creep is the high-temperature deformation of a material as a function of time. Other high-temperature properties related to creep are stress and modulus relaxation, inter-nal friction, and grain boundary relaxation. The creep rate increases strongly with temperature, and is often proportional to the applied stress. Microstructure (grain size and porosity) influences the creep rate; other influences are lattice defects, stoichiometry, and environment. Thus, creep rates are strongly dependent on sample history and the specific experimental method used to measure them, so the only meaningful quantitative comparison of creep rates can be made for samples with the same histories and measurement method. Some torsional creep rates of different oxides are given in Table 11 to show the wide variability of creep values. Compared with some other high temperature materials such as mullite (3Al
has a higher creep rate, which sometimes limits its application at high temperatures (above about 1,500C). See  for a review of creep in ceramics and  for a review of creep in ceramicmatrix composites.
5.6 Plastic Deformation
At high temperatures (above about 1,200C) alumina can deform by dislocation motion. The important paper by Merritt Kronberg , see also , p. 32, and , showed the details of dislocation motion in alumina. Basal slip on the close-packed oxygen planes is most common in alumina, with additional slip systems on prism planes.
Table 9 Knoop hardness of alumina as a function of temperature
T (K) Hardness (kg mm2)
400 1,950600 1,510800 1,1201,000 6801,200 4301,400 2601,600 160
Table 10 Knoop hardness values of some ceramics at 25C from [2, 22]
Material Hardness (kg mm2)
Diamond 8,500Alumina 3,000Boron carbide 2,760Silicon carbide 2,480Topaz (Al
Quartz (SiO2) 820
1 Alumina 11
5.7 Fracture Toughness
The fracture toughness KIC
of a brittle material is defined as
= YSc (7)
in which S is the applied stress required to propagate a crack of depth c, and Y is a geometrical parameter. Values of K
IC are often measured for ceramics from the lengths
of cracks around a hardness indent. KIC
is not material parameter; it depends on sam-ple history and many uncontrolled factors. It is based on the Griffith equation, which gives a necessary but not sufficient criterion for crack propagation . Thus K
not a very useful quantity for defining mechanical properties of brittle material. A value of about 3.0 MPam1/2 is often found for alumina .
6 Thermal and Thermodynamic Properties
6.1 Density and Thermal Expansion
The density of alpha alumina at 25C is 3.96 g cm3, which gives a specific volume of 25.8 cm3 mol1 or 0.0438 nm3 per Al
3 molecule. Densities of other aluminas are
given in Table 12.The coefficient of thermal expansion a of alumina at different temperatures is
given in Table 13. Often an average value of a is given over a range of temperatures, but the slope of a length vs. temperature plot at different temperatures is a more accu-rate way of describing a.
6.2 Heat Capacity (Specific Heat) and Thermodynamic Quantities
The specific heat, entropy, heat and Gibbs free energies of formation of alumina are given in Table 14, from . Above 2,790K, the boiling point of aluminum, there is a discontinuous change in the heat of formation of alumina.
Table 11 Torsional creep rates of some polycrystalline oxides at 1,300C and 124 MPa applied stress (from , p. 755)
Material Creep rate (105 h1)
BeO 30MgO (slip cast) 33MgO (pressed) 3.3MgAl
4, spinel (25 m grains) 26
4 (13 m grains) 0.1
12 R.H. Doremus
Table 12 Densities of anhydrous and hydrated aluminas
Material Density (g cm2)
Al(OH)3 gibbsite 2.42
AlOOH diaspore 3.44AlOOH boehmite 3.01
Table 13 The coefficient of linear thermal expansion of alumina as a function of temperature
Temp. (C) da /dT (106 per C)1,000 12.0800 11.6600 11.1400 10.4200 9.1100 7.750 6.5
Table 14 Specific heat and thermodynamic properties of -alumina as a function of temperatureSpecific heat Entropy Heat of formation Free energy of formation
T (K) J mol1 K1 kJ mol1
0 0 0 1663.608 1663.608100 12.855 4.295 1668.606 1641.692200 51.120 24.880 1673.388 1612.636298.15 79.015 50.950 1675.692 1582.275400 96.086 76.779 1676.342 1550.226600 112.545 119.345 1675.300 1487.319800 120.135 152.873 1673.498 1424.9311,000 124.771 180.210 1693.394 1361.4371,200 128.252 203.277 1691.366 1295.2281,400 131.081 223.267 1686.128 1229.3931,600 133.361 240.925 1686.128 1163.9341,800 135.143 256.740 1683.082 1098.8412,000 136.608 271.056 1679.858 1034.0962,200 138.030 284.143 1676.485 969.6812,327 138.934 291.914 Melting temperature2,400 139.453 296.214 1672.963 905.5822,600 140.959 307.435 1669.279 841.7812,800 142.591 317.980 2253.212 776.3353,000 144.474 327.841 2244.729 671.139
1 Alumina 13
6.3 Vaporization of Alumina
There is a detailed discussion of the vaporization behavior of alumina and other oxides in . The main vapor species over alumina are Al, AlO, Al
2O, and AlO
depending on the temperature and oxidizing or reducing conditions in the surrounding atmosphere. Under reducing conditions Al and Al
2O are predominant; in 0.2 bar O
both AlO and AlO2 are the main species .
Two examples of quantitative data of vapor pressure as a function of temperature are given in Table 15.
The boiling temperature of alumina at one atm pressure is about 3,530C with a heat of vaporization of about 1,900 kJ mol1 at 25C , when compared with the melting temperature of 2,054C, and a heat of fusion of about 109 kJ mol1 at 25C .
6.4 Thermal Conductivity
The thermal conductivity of -alumina single crystals as a function of temperature is given in Table 16 (from [2, 23]). Heat is conducted through a nonmetallic solid by lat-tice vibrations or phonons. The mean free path of the phonons determines the thermal conductivity and depends on the temperature, phononphonon interactions, and scat-tering from lattice defects in the solid. At temperatures below the low temperature maximum (below about 40K), the mean free path is mainly determined by the sample size because of phonon scattering from the sample surfaces. Above the maximum, the
Table 15 The pressure of AlO vapor and total vapor pressure in equilibrium with -Al
3 as a function of temperature, for
reducing and neutral conditions
Log vapor pressure ofTemp. (K) AlO, P (bar) 
1,520 151,630 131,750 111,900 92,020 72,290 5
Temp. (K) Log total vapor pres- sure, P (atm.) [2, 31]
2,309 5.062,325 4.992,370 4.782,393 4.772,399 4.662,459 4.422,478 4.242,487 4.042,545 3.702,565 3.892,605 3.72
14 R.H. Doremus
conductivity decays approximately exponentially because of phononphonon interac-tions. At high temperatures (above about 800C), the phonon mean free path is of the order of a lattice distance, and becomes constant with temperature. There is a much more detailed discussion of phonon behavior in ceramics and glasses in [23, 32]. The velocity v of a phonon or sound wave in a solid can be found from the formula
v2 = E/r (8)
in which E is Youngs modulus and r is the density, so this velocity in alumina is 10.1(10)3 m s1 at 25C. This result is close to the measured value of 10.845 m s1.
7 Electrical Properties
7.1 Electrical Conductivity
There have been a large number of studies of electrical conductivity of alumina, with widely different values being reported. Papers before 1961 are listed in  and those from 1961 to 1992 in .
Anyone interested in the electrical conductivity of alumina should read carefully the papers of Will et al. . These authors measured the electrical conductivity of highly pure and dry sapphire from 400C to 1,300C; the elemental analysis of their sapphire samples is given in Table 17, and showed less than 35 ppm total impurities. Particularly significant is the low level of alkali metal impurities, which often provide ionic conduction in oxides.
The measurements in  were made with niobium foil electrodes with a guard ring configuration on disc samples, and in a vacuum of 107108 Torr. A nonsteady-state voltage sweep technique was used for the measurements. The results are in Table 18 and Fig. 3 for conductivity along the x-axis. Between 700C and 1,300C, the activation energy was about 460 kJ mol1 (4.8 eV) and between 400 and 700C it was 39 kJ mol1
(0.4 eV). The great care taken with these measurements and the high purity of the sapphire make them definitive for the electrical conductivity for pure, dry alumina.
Table 16 Thermal conductivity of single crystal -Al2O
Conductivity ConductivityTemp. (K) (J s1 mK1) Temp. (C) (J s1 mK1)
0 0 25 3610 1,200 100 2920 3,800 300 1640 5,900 500 1050 5,000 700 7.560 2,300 900 6.380 790 1,100 5.9100 400 1,300 5.9200 100 1,500 5.4 1,700 5.9 1,900 6.3
From [2, 23]
1 Alumina 15
Table 17 Chemical analysis of sapphire for electrical conductivity measurements, from 
Element Conc. (ppm) Element Conc. (ppm)
Iron 8 Potassium
16 R.H. Doremus
The electrolysis experiments of Ramirez et al.  show that when alumina con-tains some water (OH groups), the electrical conductivity results from the transport of hydrogen ions (actually hydronium ions, H
3O+; see  for discussion).
The diffusion coefficient of H3O+ ions at 1,300C calculated  from the experi-
ments in  is 2.3(10)9 cm2 s1. This value is close to measured values of the diffu-sion coefficients of water in alumina . Thus the mechanism of the diffusion of water in alumina is the transport of H
3O+ ions, and these ions control the electrical
conductivity when the water concentration is high enough.To calculate the minimum concentration C of water in alumina that can contribute
to the electrical conductivity, one can use the Einstein equation:
C = RTs / Z 2F 2D (10)
in which R is the gas constant, Z the ionic charge (valence), F the Faraday, and D the diffusion coefficient. The electrical conductivity at 1,300C from  was 2.29
TEMPERATURE [ C]
RECIPROCAL TEMPERATURE (104 / TK)
1300120011001000 900 800 700 600 500 400
7 8 9
10 11 12 13 14 15
Fig. 3 The electrical conductivity of pure, dry sapphire along the c-axis. Points, measured values. From 
1 Alumina 17
1011/ohm cm. Thus with D = 2.29(10)9 cm2 s 1, a concentration of 1.13(10)8 mol cm3 of carriers results if one assumes that the conductivity in the samples in  results from H
3O+ transport (which, of course, it does not); this concentration is
1.45(10)7 carriers per Al atom in alumina. The concentration of H+ in the alumina samples of  can be calculated from their highly sensitive infrared absorption measurements to be about 4.7(10)7 per Al atom. Thus one can conclude that for H
concentrations above about 108 mol cm3 (3 107 ions per Al atom), there will be a contribution of these ions to the conductivity, whereas for lower H
the conductivity will be mainly electronic.The activation energy for water diffusion in alumina is about 220 kJ mol1 (2.3 eV)
from , so that many of the earlier results on electrical conductivity of alumina, for example, those summarized in , probably result from water transport at lower temperature; at higher temperatures, electronic conductivity will predominate, because of the high activation energy of intrinsic electronic conductivity. If the alumina is dry (H
3O+ concentration below 108 mol cm3) low activation energy
extrinsic electronic conduction will be dominant at lower temperatures, resulting from donor and receptor impurities in the alumina.
7.2 Dielectric Properties
The dielectric constant of alumina is given in Table 19 as a function of temperature and crystal orientation. The dielectric constant increases slightly up to 500C, and is quite dependent on orientation. Very low dielectric loss values for sapphire have been reported , but are questionable. With reasonable purity, loss tangents below 0.001 are likely. Actual values probably depend strongly on crystal purity.
7.3 Magnetic Properties
Alumina is diamagnetic with a susceptibility less than 106 .
8 Diffusion in Alumina
Experimental volume diffusion coefficients of substances in alumina are summarized in ref. 41. Values for the parameters D
0 and Q (activation energy) from the Arrhenius equation:
D = D0 exp( Q / RT ) (11)
Table 19 Dielectric constant of sapphire as a func-tion of temperature at frequencies from 103 to 109 Hz (from ). Orientation to c axis
Temp. (C) I II
25 9.3 11.5300 9.6 12.1500 9.9 12.5
18 R.H. Doremus
The fastest diffusing substance in alumina is hydrogen (H2). Fast-diffusing cations are
sodium, copper, silver, with hydroniums (H3O+) the fastest of these monovalent cati-
ons. Many other di- and trivalent cations have diffusion coefficients intermediate between these fast-diffusing ions and the slowest diffusers, the lattice elements alumi-num and oxygen, which have about the same diffusion coefficients.
A number of experimenters have calculated diffusion coefficients D from tails on diffusion profiles in alumina, and attributed these D values to diffusion along dislocations,subboundaries, or grain boundaries. However, this attribution is doubtful in most cases,as discussed in . In only two studies [43, 44] is it likely true diffusion along grain boundaries or dislocations was measured . Mechanisms of diffusion in alumina are uncertain; a variety of charged defects have been suggested to control diffusion in alumina, but no interpretation is widely accepted because of discrepancies with experimental results. I have suggested that oxygen and aluminum diffusion in alumina results from transport of aluminum monoxide (AlO), and that AlO defects in the alumina structure are important in diffusion. These speculations have some support, but need more work to confirm them.
9 Chemical Properties
The decomposition of alumina at high temperatures can be deduced from its vapor pressure; see Sect. 6.3 and Table 15.
Fig. 4 Log diffusion coefficients vs. 104/T for selected substances diffusing in alumina. From 
1 Alumina 19
9.1 Reactions with Metals
The chemical reactions of alumina with other substances can best be explored from the thermodynamic properties of these reactions. If the Gibbs free energy G of the reaction at a particular temperature is negative, the reaction tends to take place, and if G this energy is positive the reaction tends not to occur. These considerations are modified by concentrations (more properly, thermodynamic activities) of the compo-nents as expressed in an equilibrium constant of the reaction. See books on thermody-namics for more details, for example .
The relative Gibbs free energies of the reactions of metals with oxygen tell whether or not a particular metal will displace the aluminum in alumina. The reaction of aluminum with oxygen is
3Al O Al O+ =2 2 3
All of the oxidation reactions with metals are written with one mole of O2 reacting for
consistent comparison. This is the format for reactions plotted in an Ellingham dia-gram (see ). The Gibbs free energies of some of these oxidation reactions are given in Table 20, taken from [28, 29, 4648]. If the Gibbs free energy of the reaction is higher than that of aluminum (845.6 kJ mol1 for reaction (12)), then this metal will react with alumina, displacing all the aluminum in any alumina in contact with the metal, either solid, liquid, or vapor. For example for yttrium:
32 2 3Y O Y O+ = (13)
the Gibbs free energy is 1017 kJ mol1, so yttrium will displace aluminum from alumina:
2 22 3 2 3Y Al O Al Y O+ = + (14)
The free energy change of reaction 14 can be deduced from the values for Eqs. (12) and (13) from Table 20 to be 256 kJ mol1, showing the tendency for yttrium to displace aluminum. If the free energy shown in Table 20 is less than that for oxidation of aluminum, the metal will not react with alumina. Thus at 1,000C, sodium and potassiumvapors (1 atm) do not react with alumina, but 1 atm. of lithium vapor does. Liquid alkaline earths metals such as Mg, Ca, Sr, and Ba react with alumina at 1,000C and displace aluminum metal. The relative tendency of reactions of solid and liquid metals with alumina does not change much with temperature. Of course at low temperatures (below about 500C), the rates of reactions can be slow, even if the thermodynamics show a tendency to react. Gibbs free energies for other temperatures can be calculated from data in the thermodynamic tables in [28, 29, 4648].
9.2 Reactions with Nonmetals
The halides Cl2, Br
2, and I
2 do not react with alumina, but fluorine (F
2 6 4 32 3 2 3 2Al O F AlF O+ = + (15)
20 R.H. Doremus
At 1,000C the Gibbs free energy for this reaction is about 2133 kJ mol1, showing a strong tendency to react.
Reactions of the gases H2, H
2O, CO, and CO
2 with alumina can be deduced from
Al O H Al H O2 3 2 23 2 3+ = + (16)
Al O CO Al CO2 3 23 2 3+ = + (17)
At equilibrium at 1,000C the ratio of H2/H
2O is about 1010 and CO/CO
2 about 2(10)10.
It is impossible to reduce the water or carbon dioxide levels so low in any practical reaction process, so effectively H
2 and CO do not reduce Al
3. Even at 2,000C
these ratios are about 3(10)4 and 2(10)5, which are difficult levels to maintain in prac-tice. A possible reaction of alumina with carbon is
2 6 32 3 4 3 2Al O C Al C CO+ = + (18)
However, the Gibbs free energy of this reaction is +1131 kJ mol1 at 1,000C and +504.6 kJ mol1 at 2,000C, so it will take place only at very low carbon dioxide concentrations.
Other chemical reactions of alumina can be examined with the thermodynamic data in [2830, 4748].
9.3 Reactions of Alumina in Aqueous Solutions
Alumina is amphoteric, which means that it dissolves in acidic and basic solutions, but not in neutral aqueous solutions. The solubility of alumina in solutions of pH from about 49 is low; at 25C it is less than 107 mol l1 at pH 6 . Alternatively, alumina dissolves readily in strong acids (HCl, HNO
4) and strong bases (NaOH, KOH)
at temperatures well above ambient (e.g., 90C).
Table 20 Gibbs Free energies of reactions of metals with 1 atm. of oxygen at 1,000C from [28, 29, 4648]
Solid metals G (kJ mol1) Liquid metals GY 1,017 Zr 849 Ca 1,013Ti 678 CE 962Si 644 Mg 937V 619 Ba 879Mn 586 Li 870Cr 544 Al 845.6One atm. G (kJ/mol)
of metal vaporNa 444 Zn 418 K 326
Metal + O2 = oxide
1 Alumina 21
10 Optical Properties
10.1 Refractive Index
The optical properties of solids can be studied with the complex refractive index n*:
n n ik* = + (19)
in which n is the real part of the refractive index and k is the imaginary part or absorption index. Values of n and k from 0.008731 m to 600 m (142.0000.00207 eV) are given to high accuracy and many wavelengths for alumina in . In the wave-length range from 0.1454 m to 4.000 m (8.5290.31 eV), the value of k for highly pure alumina is less than 106 [49, 50], so the alumina is effectively trans-parent. Values of n for this wavelength range are given to four significant figures in Table 21. Values of n in the fifth or sixth significant figure are different for different investigations, probably because of different purities of samples and different measuring techniques and errors. A two-term equation for n (ordinary ray) in this wavelength range is 
n = +
1 744530 0101
with l the wavelength in micrometers. This equation gives n accurately to about four significant figures (Table 21). A more accurate three-term Sellmeier equation is
nA A A2 1
with the constants Ai and
i given in Table 22.
10.2 Optical Absorption
The absorption limit of 8.73 eV in Table 23 is close to the band gap of 8.8 eV for alu-mina. At energies lower than 8.73 eV, trace impurities and defects in the alumina lead to absorption tails as described in . Values of n and k at higher energies than 8.73 eV are given in Table 23 to three or four significant figures. Values from different research groups can vary substantially ; those in Table 23 are from . See  for n and k values at many more energies (wavelengths).
The values of k in Table 23 show a maximum at about 13 eV, which can be attributed to exitonic absorption ; other electronic processes in the ultra-violet spectral range are also described in .
Appreciable absorption begins in the infrared spectral range above a wavelength of 4.0m, as shown in Table 24; there are absorption peaks at 17.24 m (580 cm1) and 22.73m (440 cm1), which result from lattice vibrations. For more details see .
The optical anisotropy of alumina results in slightly different n and k values for the ordinary and extraordinary ray, as shown in detail in  (see Table 22). This anisot-ropy is related to the hexagonal (rhombohedral) structure of the alumina.
22 R.H. Doremus
The refractive index of alumina increases slightly with increasing temperature T in the visible and near-visible spectral range. The value of the temperature coefficient dn/dT of the refractive index from wavelengths 0.40.8 m is about 13(10)6K1 .
10.3 Color of Alumina
Without impurities alumina is colorless. However, addition of transition metal ions to alumina leads to spectacular colors, gem stones, and practical applications such as ruby lasers. Many aspects of color are discussed in detail in .
With the addition of about 1% of Cr2O
3 to Al
3 (replacement of one out of one
hundred of the aluminum ions with chromium ions), alumina acquires a beautiful red color and is known as ruby, one of the most prized gem stones. The red color results from transitions of electrons between energy levels in the ruby, as described in , p. 8Iff. Ruby also shows a bright red fluorescence when it is illuminated with ultra-violet light (energy of 45 eV). Ruby also shows pleochoism (multicolors); in polar-ized light the color changes as the ruby crystal is rotated .
Table 22 Refractive index , constants at 20C from 0.2 to 5.5 mm, from [49, 50]
Term Ordinary ray Extraordinary ray
l1 0.0726631 0.0740298
l2 0.1193242 0.1216529
l3 18.028251 20.072248
A1 1.4313493 1.5039759
A2 0.65054713 0.5506141
A3 5.3414021 6.5927379
Table 21 Refractive Index of sapphire at 25C in the spectral range where k < 106, from [49, 50]
Wavelength, , (m) Refractive index, n Wavelength, (m) Refractive index, n0.1464 2.231 1.367 1.7490.1603 2.070 1.530 1.7470.1802 1.947 1.709 1.7430.200 1.913 1.960 1.7380.220 1.878 2.153 1.7340.240 1.854 2.325 1.7310.260 1.838 3.244 1.7040.280 1.824 3.507 1.6950.300 1.815 3.707 1.6870.330 1.804 4.000 1.6750.361 1.794 0.405 1.786 0.436 1.781 0.486 1.775 0.546 1.771 0.579 1.769 0.644 1.765 0.707 1.763 0.852 1.759 0.894 1.758 1.014 1.755
1 Alumina 23
Table 23 Refractive index, n, and absorption index, k, of the ordinary ray for sapphire in the ultra-violet spectral range, at 25C, from [49, 50]
Energy (eV) Wavelength, l, (m) n k142.000 0.008731 0.975 0.0130120.000 0.010330 0.972 0.0177100.206 0.01237 0.892 0.08879.996 0.01550 0.929 0.13060.001 0.02066 0.911 0.13642.000 0.02952 0.859 0.09830 0.04133 0.841 0.36727.013 0.04590 0.605 0.31724.113 0.05142 0.524 0.54219.992 0.06202 0.800 0.98318.008 0.06885 1.028 1.09315.475 0.08012 1.142 1.12513.582 0.09129 1.375 1.43412.972 0.09558 2.581 1.57312.361 0.1003 1.981 1.47611.263 0.1101 2.400 1.13110.292 0.1205 2.441 0.8319.523 0.1302 2.559 0.6868.852 0.1401 2.912 0.1258.791 0.1410 2.841 0.0378.760 0.1415 2.797 0.0118.730 0.1420 2.753 0
Table 24 Refractive index, n, and absorption index, k, of the ordinary ray for sapphire in the infrared spectral range, at 25C, from 
Wavelength, l, (m) n k 4.000 1.675 1.30 (10)6
5.000 1.624 3.76 (10)5
7.143 1.459 3.60 (10)3
10.00 0.88 0.053 10.99 0.27 0.224 12.05 0.08 1.04 12.99 0.07 1.57 14.93 0.10 2.96 16.13 0.47 3.56 16.95 0.75 6.30 17.24 1.69 11.28 17.86 9.10 1.53 19.23 3.82 0.115 20.00 2.64 0.106 22.73 10.08 14.01 25.00 4.64 0.156 30.30 3.95 0.0145 33.33 3.69 0.00668 50.00 3.26 0.0117 60.13 3.19 0.0130 82.71 3.13 0.0085 100.0 3.12 0.0070 200.0 3.08 0.0035 333.3 3.07 0.0027 600.0 3.05 0.0015
24 R.H. Doremus
The deep blue color or sapphire gems results from the addition of a few hundredths of one percent of iron and titanium impurities to alumina. The Fe2+ and Ti4+ ions sub-stitute for aluminum in the sapphire, and when light of energy of 2.11 eV is shone on the sapphire, it is absorbed by the charge transfer reaction:
Fe Ti Fe Ti2 4 3 3+ + + ++ = + (22)
See , p. 140ff for a complete description of this process.A variety of other colors are found in natural and synthetic alumina crystals [2, 51].
For example, an orange-brown color is produced by Cr4+ (padparadscha sapphire) ; different transition metal ions in different concentrations and oxidation states produce many colors.
11 Conclusion and Future Uses of Alumina
The properties of alumina listed in Sects. 410 show the unusual performance of pure alumina, leading to the variety of applications given in Table 1. Practical aluminas with impurities and defects have somewhat degraded properties, but often are superior to many other materials, and have a variety of specialized applications such as refractories, electronic components, and catalyst substrates. In  there are articles discussing the future of alumina. There will continue to be incremental improvements in processing methods and properties, leading to expansion of present applications. What really new areas of application of alumina are likely? These predictions are speculative, but the most promising new applications of alumina will probably be in electronic circuits, optical components, and biomaterials. Alumina fibers for compos-ites and optics are attractive if they can be made pure, defect-free, and cheap. Because of its excellent properties other unsuspected applications of alumina will undoubtedly be developed.
1. L.D. Hart (ed.), Alumina Chemicals, The American Ceramic Society, Westerville, OH, 1990. 2. W.H. Gitzen, Alumina as a Ceramic Material, The American Ceramic Society, Westerville, OH,
1970. 3. Emphasizes defects and interfaces, especially grain boundaries, in alumina, J. Am. Ceram. Soc.
77,  (1994). 4. Emphasizes grain boundaries, grain growth, and diffusion in alumina, J. Am. Ceram. Soc. 86 
(2003). 5. P. Richet, J.A. Xu, and H.K. Mao, Quasi-hydrostatic compression of ruby to 500 kbar, Phys.
Chem. Min. 16, 207211 (1988). 6. A.P. Jephcoat, R.J. Hemley, H.K. Mao, and K.A. Goettel, X-ray diffraction of ruby (Al
to 175 GPa, Physica B 150, 115121 (1988). 7. K.T. Thomson, R.M. Wentzcovitch, and M.S.T. Bukowinski, Polymorphs of alumina predicted by
first principles, Science 274, 18801882 (1996). 8. A.H. Carim, G.S. Rohrer, N.R. Dando, S.Y. Tzeng, C.L. Rohrer, and A.J. Perrotta, Conversion of
diaspore to corundum, J. Am. Ceram. Soc. 80, 267780 (1997). 9. R.L. Coble, Transparent Alumina and Method of Preparation, U.S. Patent 3,026,210, March 20 (1967).
1 Alumina 25
10. F.J. Klug, S. Prochazka, and R.H. Doremus, Alumina-silica phase diagram in the mullite region, J. Am. Ceram. Soc. 70, 750759 (1987).
11. E.N. Bunting, Phase equilibrium in the system Cr3O3Al2O3, Bur. Stand. J. Res. 6, 947949 (1931).12. E.M. Levin, C.R. Robbins, and H.F. McMurdie, Phase Diagrams for Ceramists, Vol. IXIII, The
American Ceramic Society, 19642002.13. D.M. Roy and R.E. Barks, Subsolidus phase equilibrium in Al2O3Cr2O3, Nature, 235, 118119
(1972).14. C. Greskovich and J.A. Brewer, Solubility of magnesia in polycrystalline alumina at high tem-
peratures, J. Am. Ceram. Soc. 84, 420425 (2001).15. J.H. Gieske and G.R. Barsch, Pressure dependence of the elastic constants of single crystalline
aluminum oxide, Phys. Status Solidi 29, 121131 (1967).16. A. Kelly, Strong Solids, Chap. 1, Oxford University Press, London, 1973.17. S.M. Wiederhorn in Mechanical and Thermal Properties of Ceramics, J.B. Wachtman, (ed.), NBS
Special Publications 303, U.S. GPO, Washington, D.C., 1969, p. 217.18. R.H. Doremus, Cracks and energy-criteria for brittle fracture, J. Appl. Phys. 47, 18331836
(1976).19. R.H. Doremus, Fracture statistics: A comparison of the normal, Weibull and type I extreme value
distributions, J. Appl. Phys. 54, 193201 (1983).20. S.C. Carniglia, Reexamination of experimental strength vs. grain size data for ceramics,
J. Am. Ceram. Soc. 55, 243 (1972).21. J.E. Burke, R.H. Doremus, W.B. Hillig, and A.M. Turkalo, Static Fatigue in Glasses and Alumina,
in Materials Sci. Res. Vol. 5, W.W. Kriegel (ed.), Plenum Press, New York, 1971, pp. 435444.22. N.W. Thibault and H.Z. Nyquist, The measured Knoop hardness of hard substances and factors
affecting its determination, Trans. Am. Soc. Metals 38, 271330 (1947).23. W.D. Kingery, H.K. Bowen, and D.R. Uhlmann, Introduction to Ceramics, Wiley, New York
(1976).24. W.R. Cannon and T.G. Langdon, Creep of Ceramics, J. Mater. Sci. 18, 150 (1983); 23, 120
(1988).25. A.H. Hynes and R.H. Doremus, Theories of creep in ceramics, Crit. Rev. Solid State Mater. Sci.
21, 159 (1996).26. M.L. Kronberg, Plastic deformation of single crystals of sapphire: Basal slip and twinning, Aeta
Met. 5, 507529 (1957).27. J.D. Snow and A.H. Heuer, Slip systems in Al2O3, J. Am. Ceram. Soc. 56, 153157 (1973).28. M.W. Chase, NIST JAVAF Thermochemical Tables, J. Phys. Chem. Ref. Data, Monograph 9.29. R.H. Tamoreaux, D.L. Hildenbrand and L. Brewer, High temperature vaporization behavior of
oxides, J. Phys. Chem. Ref. Data 16, 412 (1987).30. L. Brewer and A.W. Searcy, Gaseous species of the AlAl
3 system, J. Am. Chem. Soc. 73,
53085314 (1951).31. R.V. Gains, H.C.W. Skinner, E.E. Foord, B. Mason, and A. Rosenzweig, Danas New Mineralogy,
Wiley, New York, 1977, p. 214.32. E. Schreiber and O.L. Anderson, Pressure derivatives of the sound velocities of polycrystalline
alumina, J. Am. Ceram. Soc. 49, 184190 (1966).33. J. Pappis and W.D. Kingery, Electrical properties of single and polycrystalline alumina at high
temperatures, J. Am. Ceram. Soc. 44, 459 (1961).34. F.G. Will, H.G. Lorenzi, and K.H. Janora, J. Am. Ceram. Soc. 75, 295304, 27902791 (1992).35. O.T. zkan and A.J. Moulson, The electrical conductivity of single crystal and polycrystalline
aluminum oxide, British J. Appl. Phys. 3, 983 (1970).36. H.P.R. Frederike and W.R. Hosler, High temperature electrical conductivity of aluminum oxide,
Mater. Sci. Res. 9, 233 (1973).37. K. Kituzawa and R.L. Coble, Electrical conduction in single crystal and polycrystalline Al2O3 at
high temperature, J. Am. Ceram. Soc. 57, 245 (1979).38. H.M. Kizilyalli and P.R. Mason, DC and AC electrical conduction in single crystal alumina, Phys.
Status Solidi 36, 499 (1976).39. E.E. Shpilrain, D.N. Kagan, L.S. Barkhatov, and L.I. Zhmakin, The electrical conductivity of
alumina near the melting point, High Temperatures High Pressures 8, 177 (1976).40. R. Ramirez, R. Gonzalez, J. Colera, and Y. Chen, Electric-field-enhanced diffusion of deuterons
and protons in -Al2O3 crystals, Phys. Rev. B 55, 237242 (1997).41. R.H. Doremus, Diffusion in Alumina, J. Appl. Phys. 101, 101301 (2006).
26 R.H. Doremus
42. J.D. Fowler, D. Chandra, T.S. Elleman, A.W. Payne, and K. Verghese, Tritium diffusion in Al2O3 and BeO, J. Am. Ceram. Soc. 60, 55 (1977).
43. V.S. Stubican and J.W. Orenbach, Influence of anisotropy and doping on grain-boundary diffusion in oxide systems, Solid State Ionics 12, 375 (1984).
44. X. Tang, and K.P.D. Lagerof, and A.H. Heuer, Determination of pipe diffusion coefficients in undoped and magnesia doped sapphire (-Al2O3); a study based on annihilation of dislocation dipoles, J. Am. Ceram. Soc. 86, 560565 (2003).
45. D.R. Gaskell, Introduction to the Thermodynamics of Materials, 4th edn.,Taylor and Francis, New York, 2003.
46. L.S. Darken and N.W. Gurry, Physical Chemistry of Metals, McGraw-Hill, New York, 1953.47. A. Paul, Chemistry of Glasses, Chapman and Hall, London, 1982, p. 157.48. R.H. Doremus, Diffusion of Reactive Molecules in Solids and Melts, Wiley, New York, 2002, pp.
71, 191.49. M.E. Thomas and W.J. Tropf in Handbook of Optical Constants of Solids III, E.D. Palik
(ed.), Academic Press, New York, 1998, p. 653.50. L.H. Malitson and M.J. Dodge, Refractive index and birefringence of synthetic sapphire, J. Opt.
Soc. Am. 62, 1405 (1972).51. K. Nassau, The Physics and Chemistry of Color, Wiley, New York, 1983.
J.F. Shackelford and R.H. Doremus (eds.), Ceramic and Glass Materials: 27Structure, Properties and Processing. Springer 2008
David J. Duval, Subhash H. Risbud, and James F. Shackelford
Abstract Mullite is the only stable intermediate phase in the aluminasilica system at atmospheric pressure. Although this solid solution phase is commonly found in human-made ceramics, only rarely does it occur as a natural mineral. Yet mullite is a major component of aluminosilicate ceramics and has been found in refractories and pottery dating back millennia. As the understanding of mullite matures, new uses are being found for this ancient material in the areas of electronics and optics, as well as in high temperature structural products. Many of its high temperature properties are superior to those of most other metal oxide compounds, including alumina. The chemical formula for mullite is deceptively simple: 3Al
2. However, the phase
stability, crystallography, and stoichiometry of this material remain controversial. For this reason, research and development of mullite is presented in an historical perspec-tive that may prove useful to engineers and scientists who encounter this material under nonequilibrium conditions in their work. Emphasis is placed on reviewing studies where the primary goal was to create single-phase mullite monoliths with near theoretical density.
Mullite is a solid solution phase of alumina and silica commonly found in ceramics. Only rarely does mullite occur as a natural mineral. According to introductory remarks made by Schneider and MacKenzie at the conference Mullite 2000, the geologists Anderson, Wilson, and Tait of the Scottish Branch of His Majestys Geological Survey discovered the mineral mullite less than a century ago. The trio was collecting mineral specimens from ancient lava flows on the island of Mull off the west coast of Scotland when they chanced upon the first known natural deposit of this ceramic material. The specimens were initially identified as sillimanite, but later classified as mullite.
Being the only stable intermediate phase in the Al2O
2 system at atmospheric
pressure, mullite is one of the most important ceramic materials. Mullite has been fabricated into transparent, translucent, and opaque bulk forms. These materials may have optical and electronic device applications. Mullites temperature stability and
28 D.J. Duval et al.
refractory nature are superior to corundums in certain high-temperature structural applications. Another characteristic of this aluminosilicate is its temperature-stable defect structure, which may indicate a potential use in fuel cell electrolytes.
In this chapter, developments in the understanding of mullite over the last few decades are reviewed. A discussion of crystal structures and phase stability is pre-sented to provide the reader with an overview of certain characteristics of this mate-rial. The next part of this chapter examines the effect of process chemistry on the synthesis and microstructure of mullite. The role of various synthetic methods that are used to modify mullite formation will be discussed, followed by a compilation of selected materials properties.
2 Crystal Structure
The X-ray diffraction pattern of mullite is very similar to that of sillimanite. Sillimanite is a commonly occurring aluminosilicate mineral stable at high pressures with the chemical formula Al
10, a 1:1 ratio of silica to alumina.
Roughly speaking, the sillimanite and mullite structures consist of chains of dis-torted edge-sharing AlO octahedra at the corners and center of each unit cell running parallel to the c-axis. The chains are cross-linked by SiO and AlO corner-sharing tetrahedra . Mullite is a solid solution compound with stoichiometries ranging from relatively silica-rich 3Al
2 (3:2 mullite) to alumina-rich 2Al
mullite). The structure of mullite is summarized in Table 1. Some authors use the Al/Si ionic ratio when referring to mullite stoichiometry. In this case, 3:2 mullite would have an aluminum/silicon ionic ratio of 3:1. To avoid further confusion and follow the convention most commonly used in the literature, mullite stoichiometry will be based on the alumina/silica molecular ratio. The chemical formula for mullite is often given by Al
10x, where x = 0 corresponds to sillimanite, x = 0.25 corresponds
Table 1 Wyckoff positions and coordinates of atom sites for the orthorhombic mullite structure with space group Pbam (No. 55)
Lattice parameters a = 0.75499(3) nm b = 0.76883(3)nm c = 0288379(9) nm
2a 4h 4h 2d 4h 4h 4g
Coordinatex 0 0.1474(6) 0.268(3) 0.5 0.451(5) 0.3566(6) 0.1263(9)y 0 0.3410(6) 0.207(2) 0.0 0.048(5) 0.4201(6) 0.2216(8)z 0 0.5 0.5 0.5 0.5 0.5 0.0
Thermal parameter (b)
0.5(1) 0.3(1) 1.2(8) 0.8(1) 0.8(1) 0.8(1) 0.8(1)
Occupancy O 1 0.5 0.166(7) 0.5 0.166(7) 1 1 Al 0.334(7) Si
The chemical formula is Al2(Al
10x, where x = 0.33 and the calculated density is 3.16 g
cm3. From 
2 Mullite 29
to 3:2 mullite, and x = 0.4 corresponds to 2:1 mullite. Diffusion studies  have shown that the following chemical formula is more appropriate even though it is not com-monly seen in the literature:
A1 A1 Si OVI IV43
The symbol denotes an oxygen vacancy. The superscripts VI and IV indicate octa-hedral and tetrahedral coordination sites, respectively.
With increasing alumina content, Si4+ is replaced by Al3+ and anion (oxygen) vacan-cies are created to maintain charge neutrality. Accommodating the structural defects causes significant distortions of the aluminum and silicon polyhedra. In mullite (as opposed to sillimanite), there are three (as opposed to four) tetrahedral chains in the unit cell, with a somewhat random distribution for silica and alumina tetrahedra . This results in the necessity for distorted alumina tetrahedra to be arranged in an oxygen-deficient tricluster (three tetrahedra sharing single corner-bridging oxygen). These clusters constitute a distinctive element of mullites crystal structure [2,5].
Unlike sillimanite, X-ray diffraction patterns of mullite exhibit significant dif-fuse scattering and possible superlattice reflections. Authors have proposed various models to account for mullites anomalous scattering using superlattice refinement, atomic site occupancy factor calculation, and correlated vacancy mapping [2,6,7]. Most work suggests that defects tend to cluster or correlate with short-range order along specific crystallographic directions. Lower alumina concentrations result in less directional correlation of oxygen vacancies or more random vacancy distribu-tions. According to Freimann and Rahman , oxygen vacancies tend to correlate parallel with the lattice parameter a, and to a lesser extent with b. The authors suggest their correlation results could be used to interpret thermal expansion behavior of mullites. As a practical matter, the lattice parameter a correlates linearly with
Fig. 1 Structure of mullite. (a) Average structureand (b) atomic displacements around an oxygen vacancy. From 
AI*O - vacancy
Si / AI (Tetr.)
30 D.J. Duval et al.
3 content. Figure 1 depicts the mullite unit. Atom positions for an intermediate
composition of mullite, Al2(Al
10x, where x = 0.33 are provided in Table 1.
X-ray powder diffraction patterns demonstrating mullite crystallization from amorphous precursors are shown in Fig. 2 .
It should be noted that there is no convincing evidence of mullite formation in regions of the phase diagram with compositions between 3:2 mullite and sillimanite. In other words, the chemical formula for mullite cannot accommodate x values such that 0 < x< 0.25. Although the presence of a cubic spinel with the stoichiometry and structure similar to that of 2:1 mullite had been reported [9,10], its existence is likely of academic rather than practical significance. What was originally reported as a tetragonal phase of 3:1 mullite  formed by rapid quenching of the melt could be attributed to severe microtwinning of the usual orthorhombic structure . On the other hand, workers have recently reported mullite phases with Al
2 ratios up to and greater than 9:1
. These specialty compounds are potentially useful in specific refractory appli-cations due to their high Al
3 content. Unfortunately, it has proved difficult to produce
these ultra-high alumina mullites in sufficient quantity and purity. Further research is required before practical applications for these materials can be envisioned.
3 Phase Stability
An historical perspective may prove useful to engineers or scientists who encounter mullite during the course of their work: The earliest interpretations of the materials behavior may reflect the result of nonequilibrium conditions that often occur in production or experimental situations.
Fig. 2 X-ray powder diffraction patterns showing the crystallization of mullite from amorphous precursors as a function of temperature. M denotes mullite peaks, and Sp markers denote the inter-mediate -Al
3 spinel peaks. From 
Degree 220 30 40 50 60 70 80
sp spsp sp
2 Mullite 31
Mullite-based ceramics have been widely used as refractories and in pottery for millennia. Although the technology of mullite is becoming more mature, there are still questions concerning its melting behavior and the shape of mullite phase boundaries in the Al
2 phase diagram. In 1924, Bowen and Grieg  published the first
phase diagram to include mullite as a stable phase, but did not indicate a solid solution range. The phase 3Al
2 was reported to melt incongruently at 1,810C.
Specimens were prepared from mechanical mixtures of alumina and silica melted and quenched in air. Shears and Archibald  reported the presence of a solid solution range from 3Al
2 (3:2 mullite) to 2Al
2 (2:1 mullite) in 1954. Their
phase diagram depicted a mullite solidus shifting to higher alumina concentrations at temperatures above the silicamullite eutectic temperature.
In 1958, Toropov and Galakhov  presented a phase diagram where mullite was shown to melt congruently at 1,850C. Aramaki and Roy  published a phase dia-gram in 1962 corroborating a congruent melting point for mullite at 1,850C. Their specimens were prepared from gels for subsolidus heat treatments, while mechanical mixtures of -Al
3 and silica glass were prepared for heat treatments above the
solidus temperature. Specimens were encapsulated to inhibit silica volatilization. A silicamullite eutectic temperature of 1,595C and a mullitealumina eutectic temperature of 1,840C were reported. No shift in the mullite solidus phase boundary with temperature was reported in either of these publications.
Over a decade later, Aksay and Pask  presented a different phase diagram depicting incongruent melting for mullite at 1,828C. Specimens, in the form of dif-fusion couples between sapphire and aluminosilicate glass, were also encapsulated to inhibit volatilization. Many authors suggest that nucleation and growth of mullite occurs within an amorphous alumina-rich siliceous phase located between the silica and alumina particles . On the other hand, Davis and Pask  and later Aksay and Pask observed coherent mullite growth on sapphire in a temperature range from about 1,600 to below 1,800C, indicating interdiffusion of aluminum and silicon ions through the mullite . Risbud and Pask  later modified the diagram to incorporate metastable phase regions. They showed a stable silicamullite eutectic temperature of 1,587C. An immiscibility dome with a spinodal region was reported between approximately 7 and 55 mol% Al
3. The dome has a central composition of
about 35 mol% Al2O
3, and complete miscibility occurs near 1,550C (temperatures
below the silicamullite eutectic temperature). A stable mullitealumina peritectic was reported at 1,828C. However, a metastable incongruent melting point for mul-lite was reported at 1,890C. The metastable mullite compositions were shifted toward higher alumina concentration. To account for the metastability, the authors suggested there could be a barrier for alumina precipitation in both melt and mullite, and that mullite could be superheated. Figure 3 portrays this phase diagram showing regions of metastability .
In 1987, Klug et al. published their SiO2Al
3 phase diagram . They reported
incongruent melting for mullite at 1,890C, and shifting of both boundaries of the mullite solid solution region toward higher alumina content (2:1 mullite) at tempera-tures above the eutectic point of 1,587C. This phase diagram appears to reconcile most of the phenomena observed by other workers on the SiO
Seemingly irreconcilable observations involving phase stability of similarly prepared specimens have been attributed convincingly to nonequilibrium conditions and/or sil-ica volatilization. This phase diagram  is shown in Fig. 4.
32 D.J. Duval et al.
The 2:1 mullite appears to be only metastable at room temperature , and very high temperature use or cycling might cause some alumina to precipitate. However, Pask  suggested that discrepancies in the reported behavior of mullite are attributa-ble to the presence or absence of -Al
3 in the starting materials. Engineers or scien-
tists are cautioned to use the appropriate phase diagram consistent with their experimental methods and conditions. It should also be noted that at tectonic pressures, SiO
exsolve from mullite leaving a compound with a stoichiometry Al2O
on temperature and pressure, the compound will be sillimanite, kyanite, or andalusite.
4 Processing and Applications
As mentioned in the previous section, the formation, phase purity, and morphology of mullite depend upon precursor materials and processing history. Mullite was first identified as the product of heating kaolinitic clays, resulting in a compound with an
Fig. 3 The system Al2O
2 showing metastable regions. The gaps shown with spinodal regions
are considered the most probable thermodynamically. From 
2 Mullite 33
approximate alumina-to-silica molar ratio of 3:2. The order of reaction proceeds as follows :
4 450C 2(Al
2) + 2H
2) 925C 2Al
2 + SiO
Metakaolin Silicon spinel
2 1,100C 2(Al
2) + SiO
Silicon spinel Pseudomullite
2) 1,400C 3Al
2 + SiO
Pseudomullite Mullite + cristobalite
Excess corundum may be added, and the system heated at higher temperatures to minimize free SiO
2. Toward this end, Goski and Caley  suspended grains of the
mineral kyanite (a high-pressure form of Al2O
2) with submicron alumina in
water to provide intimate mixing of these mullite precursors. The aluminakyanite suspension was slip cast to form a green body that was reaction-sintered to form an aluminamullite composite. According to phase diagrams, a silica-rich glassy phase in 3:2 mullite is predicted when sintered at temperatures higher than the eutectic (1,587C). Many common 3:2 mullite products are sintered between 1,600 and 1,700C and may contain a glassy phase in the microstructure.
Fig. 4 Phase diagram for the aluminasilica system. From 
SiO2 + MULLITE
0 20 4030 50 60 70 80 90 100
100 20 4030 50 60 70 80 90 100
34 D.J. Duval et al.
High-purity glass-free mullite monoliths have been obtained by at least three tradi-tional methods:
1. Starting materials with alumina contents near the stoichiometry of 2:1 mullite may be completely melted above 1,960C and then cooled to about 1,890C without crystallizing. At the latter temperature (in the shifted solid solution region), infrared-transparent mullite single crystals could be grown by the Czochralski method .
2. Pask  reports that mullites with higher molar ratios of alumina to silica (i.e., >3:1)have been prepared by homogenous melting of the constituents above the liquids and subsequent quenching. As a note, mullites prepared by fusion are generally weaker than those produced by sintering .
3. Mullite powders obtained by various methods can first be crystallized near 1,200C, and then sintered at temperatures below the eutectic. Highly pure mullite and mullite composites have been obtained by hot pressing below 1,300C with this method .
When processed close to or above the eutectic temperature (~1,590C), mullite with bulk compositions of less than 72 wt% Al
3 (3:2 mullite) exhibits a microstructure
of elongated grains that is believed to be promoted by the presence of a glassy second phase. For Al
3 concentrations greater than 72 wt% Al
3, the amount of glassy
phase is less and the initially formed mullite grains are smaller and more equiaxial. Further heat treatment results in rapid grain growth driven by a decrease of the high grain boundary area associated with the fine grains in the initial system. This leads to fast growth of the grains along the c-axis and a higher aspect ratio for the overall grains. After this rapid decrease in the driving force, the grains grow more slowly and the overall decrease in the free energy of the system dictates the development of a more equiaxial microstructure 
An interesting approach in making mullite powders has been via combustion syn-thesis . An aqueous heterogeneous redox mixture containing aluminum nitrate, silica fume (soot), and urea in the appropriate mole ratio is mixed together. When rapidly heated to 500C, the mixture boils, foams, and can be ignited with a flame. The process yields weakly crystalline mullite powder in less than 5 min. Fully crystal-line mullite can be obtained by incorporating an extra amount of oxidizer, such as ammonium perchlorate in the solution.
Recent work on mullite synthesis has focused on variations of solgel methods, which allow control of the local distribution and homogeneity of the precursor chemistry. The microstructure of a solgel derived mullite is shown in Fig. 5. Along with an understanding of kinetics, solge